#------------------------------------------------------------------------------
#$Date: 2017-02-07 17:13:06 +0200 (Tue, 07 Feb 2017) $
#$Revision: 191892 $
#$URL: file:///home/coder/svn-repositories/cod/cif/2/10/35/2103534.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2103534
loop_
_publ_author_name
'Pavlovska, A.'
'Werner, S.'
'Maximov, B.'
'Mill, B.'
_publ_section_title
;
 Pressure-induced phase transitions of piezoelectric single crystals
 from the langasite family: La₃Nb~0.5~Ga~5.5~O₁₄ and
 La₃Ta~0.5~Ga~5.5~O₁₄
;
_journal_issue                   6
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              939
_journal_page_last               947
_journal_paper_doi               10.1107/S0108768102010273
_journal_volume                  58
_journal_year                    2002
_chemical_formula_sum            'Ga5.54 La3 O14 Ta0.46'
_chemical_formula_weight         1110.22
_chemical_name_systematic        ?
_space_group_IT_number           150
_symmetry_space_group_name_Hall  'P 3 2"'
_symmetry_space_group_name_H-M   'P 3 2 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            1
_cell_length_a                   8.116
_cell_length_b                   8.116
_cell_length_c                   5.086
_cell_measurement_temperature    293(2)
_cell_volume                     290.1
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_pressure         5.1E+6
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.611
_diffrn_measured_fraction_theta_max 0.611
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0646
_diffrn_reflns_av_sigmaI/netI    0.0388
_diffrn_reflns_limit_h_max       11
_diffrn_reflns_limit_h_min       -11
_diffrn_reflns_limit_k_max       11
_diffrn_reflns_limit_k_min       -11
_diffrn_reflns_limit_l_max       4
_diffrn_reflns_limit_l_min       -4
_diffrn_reflns_number            1737
_diffrn_reflns_theta_full        31.95
_diffrn_reflns_theta_max         31.95
_diffrn_reflns_theta_min         2.90
_exptl_absorpt_coefficient_mu    27.826
_exptl_crystal_density_diffrn    6.354
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             488
_refine_diff_density_max         1.980
_refine_diff_density_min         -1.801
_refine_diff_density_rms         0.465
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.00(4)
_refine_ls_extinction_coef       0.155(10)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   0.716
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     39
_refine_ls_number_reflns         438
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      0.716
_refine_ls_R_factor_all          0.0336
_refine_ls_R_factor_gt           0.0335
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.1000P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0737
_refine_ls_wR_factor_ref         0.0738
_reflns_number_gt                437
_reflns_number_total             438
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            sn0021-5.1cad4.cif
_cod_data_source_block           5.1cad4
_cod_depositor_comments
;
The _diffrn_ambient_pressure was taken from the original data block
header, after comparison with the paper text and supplementary
material.

Saulius Gra\<zulis
;
_cod_database_code               2103534
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'y, x, -z'
'-y, x-y, z'
'-x+y, -x, z'
'-x, -x+y, -z'
'x-y, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
La La -0.42799(8) 0.0000 0.0000 0.0179(3) Uani 1 2 d S
Ga1 Ga 0.0000 0.0000 0.0000 0.0159(4) Uani 0.54 6 d SP
Ta Ta 0.0000 0.0000 0.0000 0.0159(4) Uani 0.46 6 d SP
Ga2 Ga -0.6667 -0.3333 0.4693(5) 0.0177(5) Uani 1 3 d S
Ga3 Ga -0.76424(15) 0.0000 -0.5000 0.0194(4) Uani 1 2 d S
O1 O -0.3333 0.3333 0.173(3) 0.020(3) Uani 1 3 d S
O2 O -0.5461(9) 0.1487(9) -0.297(2) 0.027(2) Uani 1 1 d .
O3 O -0.7812(8) 0.1452(9) 0.2426(18) 0.028(2) Uani 1 1 d .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
La La -0.2871 2.4523 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ta Ta -0.7052 6.5227 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ga Ga 0.2307 1.6083 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O3 La O3 67.7(4) 3_565 5_445
O3 La O2 108.0(3) 3_565 6
O3 La O2 140.0(3) 5_445 6
O3 La O2 140.0(3) 3_565 .
O3 La O2 108.0(3) 5_445 .
O2 La O2 99.2(4) 6 .
O3 La O1 124.1(2) 3_565 2_455
O3 La O1 79.5(2) 5_445 2_455
O2 La O1 70.8(3) 6 2_455
O2 La O1 91.9(3) . 2_455
O3 La O1 79.5(2) 3_565 .
O3 La O1 124.1(2) 5_445 .
O2 La O1 91.9(3) 6 .
O2 La O1 70.8(3) . .
O1 La O1 153.70(6) 2_455 .
O3 La O2 65.5(2) 3_565 5_445
O3 La O2 78.9(3) 5_445 5_445
O2 La O2 64.6(3) 6 5_445
O2 La O2 154.45(11) . 5_445
O1 La O2 64.7(3) 2_455 5_445
O1 La O2 126.4(3) . 5_445
O3 La O2 78.9(3) 3_565 3_565
O3 La O2 65.5(2) 5_445 3_565
O2 La O2 154.45(11) 6 3_565
O2 La O2 64.6(3) . 3_565
O1 La O2 126.4(3) 2_455 3_565
O1 La O2 64.7(3) . 3_565
O2 La O2 137.2(3) 5_445 3_565
O3 La Ga2 86.0(2) 3_565 .
O3 La Ga2 110.82(19) 5_445 .
O2 La Ga2 31.67(17) 6 .
O2 La Ga2 128.90(18) . .
O1 La Ga2 64.7(3) 2_455 .
O1 La Ga2 110.5(3) . .
O2 La Ga2 32.93(15) 5_445 .
O2 La Ga2 164.79(18) 3_565 .
O3 La Ga2 110.82(19) 3_565 2_565
O3 La Ga2 86.0(2) 5_445 2_565
O2 La Ga2 128.90(18) 6 2_565
O2 La Ga2 31.67(17) . 2_565
O1 La Ga2 110.5(3) 2_455 2_565
O1 La Ga2 64.7(3) . 2_565
O2 La Ga2 164.79(18) 5_445 2_565
O2 La Ga2 32.93(15) 3_565 2_565
Ga2 La Ga2 160.17(2) . 2_565
O3 La Ta 33.84(18) 3_565 .
O3 La Ta 33.84(18) 5_445 .
O2 La Ta 130.4(2) 6 .
O2 La Ta 130.4(2) . .
O1 La Ta 103.15(3) 2_455 .
O1 La Ta 103.15(3) . .
O2 La Ta 68.60(14) 5_445 .
O2 La Ta 68.60(14) 3_565 .
Ga2 La Ta 99.912(11) . .
Ga2 La Ta 99.913(11) 2_565 .
O3 La Ga1 33.84(18) 3_565 .
O3 La Ga1 33.84(18) 5_445 .
O2 La Ga1 130.4(2) 6 .
O2 La Ga1 130.4(2) . .
O1 La Ga1 103.15(3) 2_455 .
O1 La Ga1 103.15(3) . .
O2 La Ga1 68.60(14) 5_445 .
O2 La Ga1 68.60(14) 3_565 .
Ga2 La Ga1 99.912(11) . .
Ga2 La Ga1 99.913(11) 2_565 .
Ta La Ga1 0.0 . .
O3 Ga1 O3 106.9(4) 4_445 5_445
O3 Ga1 O3 85.7(3) 4_445 1_655
O3 Ga1 O3 163.2(4) 5_445 1_655
O3 Ga1 O3 163.2(4) 4_445 2_565
O3 Ga1 O3 85.7(3) 5_445 2_565
O3 Ga1 O3 84.3(4) 1_655 2_565
O3 Ga1 O3 84.3(4) 4_445 6_655
O3 Ga1 O3 85.7(3) 5_445 6_655
O3 Ga1 O3 106.9(4) 1_655 6_655
O3 Ga1 O3 85.7(3) 2_565 6_655
O3 Ga1 O3 85.7(3) 4_445 3_565
O3 Ga1 O3 84.3(4) 5_445 3_565
O3 Ga1 O3 85.7(3) 1_655 3_565
O3 Ga1 O3 106.9(4) 2_565 3_565
O3 Ga1 O3 163.2(4) 6_655 3_565
O3 Ga1 La 42.2(2) 4_445 2
O3 Ga1 La 98.4(2) 5_445 2
O3 Ga1 La 98.4(2) 1_655 2
O3 Ga1 La 126.5(2) 2_565 2
O3 Ga1 La 42.2(2) 6_655 2
O3 Ga1 La 126.5(2) 3_565 2
O3 Ga1 La 98.4(2) 4_445 .
O3 Ga1 La 42.2(2) 5_445 .
O3 Ga1 La 126.5(2) 1_655 .
O3 Ga1 La 98.4(2) 2_565 .
O3 Ga1 La 126.5(2) 6_655 .
O3 Ga1 La 42.2(2) 3_565 .
La Ga1 La 120.0 2 .
O3 Ga1 La 126.5(2) 4_445 4
O3 Ga1 La 126.5(2) 5_445 4
O3 Ga1 La 42.2(2) 1_655 4
O3 Ga1 La 42.2(2) 2_565 4
O3 Ga1 La 98.4(2) 6_655 4
O3 Ga1 La 98.4(2) 3_565 4
La Ga1 La 120.0 2 4
La Ga1 La 120.0 . 4
O3 Ta O3 106.9(4) 4_445 5_445
O3 Ta O3 85.7(3) 4_445 1_655
O3 Ta O3 163.2(4) 5_445 1_655
O3 Ta O3 163.2(4) 4_445 2_565
O3 Ta O3 85.7(3) 5_445 2_565
O3 Ta O3 84.3(4) 1_655 2_565
O3 Ta O3 84.3(4) 4_445 6_655
O3 Ta O3 85.7(3) 5_445 6_655
O3 Ta O3 106.9(4) 1_655 6_655
O3 Ta O3 85.7(3) 2_565 6_655
O3 Ta O3 85.7(3) 4_445 3_565
O3 Ta O3 84.3(4) 5_445 3_565
O3 Ta O3 85.7(3) 1_655 3_565
O3 Ta O3 106.9(4) 2_565 3_565
O3 Ta O3 163.2(4) 6_655 3_565
O3 Ta Ga3 97.9(2) 4_445 4_445
O3 Ta Ga3 31.5(2) 5_445 4_445
O3 Ta Ga3 160.1(2) 1_655 4_445
O3 Ta Ga3 87.2(2) 2_565 4_445
O3 Ta Ga3 54.4(2) 6_655 4_445
O3 Ta Ga3 114.0(2) 3_565 4_445
O3 Ta Ga3 31.5(2) 4_445 4_446
O3 Ta Ga3 97.9(2) 5_445 4_446
O3 Ta Ga3 87.2(2) 1_655 4_446
O3 Ta Ga3 160.1(2) 2_565 4_446
O3 Ta Ga3 114.0(2) 6_655 4_446
O3 Ta Ga3 54.4(2) 3_565 4_446
Ga3 Ta Ga3 106.08(4) 4_445 4_446
O3 Ta Ga3 54.4(2) 4_445 1_656
O3 Ta Ga3 160.1(2) 5_445 1_656
O3 Ta Ga3 31.5(2) 1_655 1_656
O3 Ta Ga3 114.0(2) 2_565 1_656
O3 Ta Ga3 97.9(2) 6_655 1_656
O3 Ta Ga3 87.2(2) 3_565 1_656
Ga3 Ta Ga3 145.011(15) 4_445 1_656
Ga3 Ta Ga3 62.76(3) 4_446 1_656
O3 Ta Ga3 114.0(2) 4_445 1_655
O3 Ta Ga3 87.2(2) 5_445 1_655
O3 Ta Ga3 97.9(2) 1_655 1_655
O3 Ta Ga3 54.4(2) 2_565 1_655
O3 Ta Ga3 31.5(2) 6_655 1_655
O3 Ta Ga3 160.1(2) 3_565 1_655
Ga3 Ta Ga3 62.76(3) 4_445 1_655
Ga3 Ta Ga3 145.011(15) 4_446 1_655
Ga3 Ta Ga3 106.08(4) 1_656 1_655
O3 Ta Ga3 87.2(2) 4_445 2_565
O3 Ta Ga3 114.0(2) 5_445 2_565
O3 Ta Ga3 54.4(2) 1_655 2_565
O3 Ta Ga3 97.9(2) 2_565 2_565
O3 Ta Ga3 160.1(2) 6_655 2_565
O3 Ta Ga3 31.5(2) 3_565 2_565
Ga3 Ta Ga3 145.010(15) 4_445 2_565
Ga3 Ta Ga3 62.76(3) 4_446 2_565
Ga3 Ta Ga3 62.76(3) 1_656 2_565
Ga3 Ta Ga3 145.010(15) 1_655 2_565
O3 Ta Ga3 160.1(2) 4_445 2_564
O3 Ta Ga3 54.4(2) 5_445 2_564
O3 Ta Ga3 114.0(2) 1_655 2_564
O3 Ta Ga3 31.5(2) 2_565 2_564
O3 Ta Ga3 87.2(2) 6_655 2_564
O3 Ta Ga3 97.9(2) 3_565 2_564
Ga3 Ta Ga3 62.76(3) 4_445 2_564
Ga3 Ta Ga3 145.010(15) 4_446 2_564
Ga3 Ta Ga3 145.010(15) 1_656 2_564
Ga3 Ta Ga3 62.76(3) 1_655 2_564
Ga3 Ta Ga3 106.08(4) 2_565 2_564
O1 Ga2 O2 118.3(3) 2_456 2_455
O1 Ga2 O2 118.3(3) 2_456 5_445
O2 Ga2 O2 99.3(4) 2_455 5_445
O1 Ga2 O2 118.3(3) 2_456 6
O2 Ga2 O2 99.3(4) 2_455 6
O2 Ga2 O2 99.3(4) 5_445 6
O1 Ga2 La 134.67(3) 2_456 4_445
O2 Ga2 La 56.1(3) 2_455 4_445
O2 Ga2 La 43.3(2) 5_445 4_445
O2 Ga2 La 106.5(3) 6 4_445
O1 Ga2 La 134.67(3) 2_456 2_455
O2 Ga2 La 43.3(2) 2_455 2_455
O2 Ga2 La 106.5(3) 5_445 2_455
O2 Ga2 La 56.1(3) 6 2_455
La Ga2 La 76.04(5) 4_445 2_455
O1 Ga2 La 134.67(3) 2_456 .
O2 Ga2 La 106.5(3) 2_455 .
O2 Ga2 La 56.1(3) 5_445 .
O2 Ga2 La 43.3(2) 6 .
La Ga2 La 76.04(5) 4_445 .
La Ga2 La 76.04(5) 2_455 .
O1 Ga2 La 41.82(3) 2_456 4_446
O2 Ga2 La 98.3(3) 2_455 4_446
O2 Ga2 La 89.1(3) 5_445 4_446
O2 Ga2 La 159.0(3) 6 4_446
La Ga2 La 92.852(5) 4_445 4_446
La Ga2 La 139.555(6) 2_455 4_446
La Ga2 La 139.555(6) . 4_446
O1 Ga2 La 41.82(3) 2_456 2_456
O2 Ga2 La 89.1(3) 2_455 2_456
O2 Ga2 La 159.0(3) 5_445 2_456
O2 Ga2 La 98.3(3) 6 2_456
La Ga2 La 139.555(6) 4_445 2_456
La Ga2 La 92.852(5) 2_455 2_456
La Ga2 La 139.555(6) . 2_456
La Ga2 La 70.54(4) 4_446 2_456
O1 Ga2 La 41.82(3) 2_456 1_556
O2 Ga2 La 159.0(3) 2_455 1_556
O2 Ga2 La 98.3(3) 5_445 1_556
O2 Ga2 La 89.1(3) 6 1_556
La Ga2 La 139.555(6) 4_445 1_556
La Ga2 La 139.554(6) 2_455 1_556
La Ga2 La 92.852(5) . 1_556
La Ga2 La 70.54(4) 4_446 1_556
La Ga2 La 70.54(4) 2_456 1_556
O3 Ga3 O3 132.7(4) 6 1_554
O3 Ga3 O2 99.5(4) 6 .
O3 Ga3 O2 109.5(3) 1_554 .
O3 Ga3 O2 109.5(3) 6 6_554
O3 Ga3 O2 99.5(4) 1_554 6_554
O2 Ga3 O2 103.1(5) . 6_554
O3 Ga3 Ta 109.6(3) 6 1_454
O3 Ga3 Ta 35.1(2) 1_554 1_454
O2 Ga3 Ta 144.4(2) . 1_454
O2 Ga3 Ta 86.2(3) 6_554 1_454
O3 Ga3 Ta 35.08(19) 6 1_455
O3 Ga3 Ta 109.6(3) 1_554 1_455
O2 Ga3 Ta 86.2(3) . 1_455
O2 Ga3 Ta 144.5(2) 6_554 1_455
Ta Ga3 Ta 106.08(4) 1_454 1_455
Ga2 O1 La 110.0(3) 2_566 .
Ga2 O1 La 110.0(3) 2_566 2_565
La O1 La 109.0(3) . 2_565
Ga2 O1 La 110.0(3) 2_566 4_455
La O1 La 109.0(3) . 4_455
La O1 La 108.9(3) 2_565 4_455
Ga2 O2 Ga3 117.4(6) 2_565 .
Ga2 O2 La 105.0(3) 2_565 .
Ga3 O2 La 120.4(3) . .
Ga2 O2 La 91.0(3) 2_565 4_455
Ga3 O2 La 112.7(3) . 4_455
La O2 La 106.0(4) . 4_455
Ga3 O3 Ta 113.4(3) 1_556 1_455
Ga3 O3 Ga1 113.4(3) 1_556 1_455
Ta O3 Ga1 0.0 1_455 1_455
Ga3 O3 La 138.2(3) 1_556 4_455
Ta O3 La 104.0(4) 1_455 4_455
Ga1 O3 La 104.0(4) 1_455 4_455
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
La O3 2.403(7) 3_565
La O3 2.403(7) 5_445
La O2 2.411(8) 6
La O2 2.411(8) .
La O1 2.569(5) 2_455
La O1 2.569(5) .
La O2 2.818(8) 5_445
La O2 2.818(8) 3_565
La Ga2 3.3953(18) .
La Ga2 3.3953(18) 2_565
La Ta 3.4735(6) .
La Ga1 3.4735(6) .
Ga1 O3 1.993(7) 4_445
Ga1 O3 1.993(7) 5_445
Ga1 O3 1.993(7) 1_655
Ga1 O3 1.993(7) 2_565
Ga1 O3 1.993(7) 6_655
Ga1 O3 1.993(7) 3_565
Ga1 La 3.4735(6) 2
Ga1 La 3.4735(6) 4
Ta O3 1.993(7) 4_445
Ta O3 1.993(7) 5_445
Ta O3 1.993(7) 1_655
Ta O3 1.993(7) 2_565
Ta O3 1.993(7) 6_655
Ta O3 1.993(7) 3_565
Ta Ga3 3.1824(8) 4_445
Ta Ga3 3.1824(8) 4_446
Ta Ga3 3.1824(8) 1_656
Ta Ga3 3.1824(8) 1_655
Ta Ga3 3.1825(8) 2_565
Ta Ga3 3.1825(8) 2_564
Ga2 O1 1.821(15) 2_456
Ga2 O2 1.846(8) 2_455
Ga2 O2 1.846(8) 5_445
Ga2 O2 1.846(8) 6
Ga2 La 3.3953(18) 4_445
Ga2 La 3.3953(18) 2_455
Ga2 La 3.6216(19) 4_446
Ga2 La 3.6216(19) 2_456
Ga2 La 3.6216(19) 1_556
Ga3 O3 1.812(8) 6
Ga3 O3 1.812(8) 1_554
Ga3 O2 1.876(8) .
Ga3 O2 1.876(8) 6_554
Ga3 Ta 3.1824(8) 1_454
Ga3 Ta 3.1824(8) 1_455
O1 Ga2 1.821(15) 2_566
O1 La 2.569(5) 2_565
O1 La 2.569(5) 4_455
O2 Ga2 1.846(8) 2_565
O2 La 2.818(8) 4_455
O3 Ga3 1.812(8) 1_556
O3 Ta 1.993(7) 1_455
O3 Ga1 1.993(7) 1_455
O3 La 2.403(7) 4_455
